**HAL Id: hal-00560311**

**https://hal.archives-ouvertes.fr/hal-00560311**

Submitted on 28 Jan 2011

**HAL is a multi-disciplinary open access**
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

### Ihor Sobchenko, Dietmar Baither, Rudolf Reichelt, Eckhard Nembach

**To cite this version:**

Ihor Sobchenko, Dietmar Baither, Rudolf Reichelt, Eckhard Nembach. Modeling and kinetic Monte Carlo simulations of the metallographic etching process of second phase particles. Philosophical Mag- azine, Taylor & Francis, 2010, 90 (05), pp.527-551. �10.1080/14786430903201846�. �hal-00560311�

**For Peer Review Only**

Modeling and kinetic Monte Carlo simulations of the metallographic etching process of second phase particles

Journal: Philosophical Magazine & Philosophical Magazine Letters Manuscript ID: TPHM-09-Apr-0140.R1

Journal Selection: Philosophical Magazine Date Submitted by the

Author: 20-Jul-2009

Complete List of Authors: Sobchenko, Ihor; Universitaetsklinikum, Institut fuer Medizinische Physik und Biophysik

Baither, Dietmar; University of Muenster, Institut fuer Materialphysik

Reichelt, Rudolf; Universitaetsklinikum, Institut fuer Medizinische Physik und Biophysik

Nembach, Eckhard; University of Muenster, Institut fuer Materialphysik

Keywords:

atomic force microscopy, chemical etching, high-resolution imaging, metallography, Monte-Carlo, nanoparticles, precipitation,

transmission electron microscopy

Keywords (user supplied): electrolytic etching, scanning electron microscopy, phase transformations

**For Peer Review Only**

PhilMagetchrev190709U

**Modeling and kinetic Monte Carlo simulations **

** of the metallographic etching process of second phase particles **

Ihor Sobchenko^{a+}, Dietmar Baither^{b}, Rudolf Reichelt^{a}, and Eckhard Nembach^{b}*

**a **Institut für Medizinische Physik und Biophysik, Universitätsklinikum,
**Universität Münster, Robert-Koch-Strasse 31, 48149 Münster, Germany **

b Institut für Materialphysik, Universität Münster, Wilhelm-Klemm-Strasse 10, 48149 Münster, Germany

+Permanent address: Department of Theoretical Physics,

Cherkasy National University, Shevchenko Blvd. 81, 18031 Cherkasy, Ukraine

*Correspondingauthor. E-mail: nembach@uni-muenster.de Phone: ++49-251-83-33570, Fax: ++49-251-83-38346

2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

**For Peer Review Only**

**Abstract **

Kinetic Monte Carlo simulations of the chemical and electrolytic etching processes of nano-scale particles in two-phase materials have been performed. Etching produces a surface relief, which can subsequently be studied by optical, scanning electron, and atomic force microscopy to obtain quantitative information on the size, shape, and spatial arrangement of the particles. The present simulations yield insight into the dependence of the etched relief on the strengths of the atomic bonds in the two phases and on the shape of the particles. Lower limits for the difference in bond energies necessary (i) to reveal the particles and (ii) to avoid over-etching are established. The results of the simulations are discussed with reference to actual etching experiments performed for nano-scale precipitates.

*Keywords: Chemical etching; electrolytic etching; metallography; Monte Carlo; nano-particles; *

precipitates; high-resolution imaging; atomic force microscopy; transmission electron microscopy;

scanning electron microscopy; phase transformations.

**1. Introduction **

The macroscopic physical properties of two- and multiphase materials are governed by two groups of parameters: (a) intrinsic properties of the constituent phases, e.g. crystal structure, electronic band structure, some dislocation parameters, saturation magnetization and (b) geometric parameters: size, shape, and spatial arrangement of the particles of the secondary phases. The latter dependence (b) is most striking in the two following examples [1]:

(i) As the average size of nano-scale coherent ductile particles in particle strengthened materials increases during ageing while the total volume fraction of the particles stays constant, the yield strength first increases with ageing time, then passes through a maximum, and finally decreases. This sequence of states is referred to as the under-, peak-, and over-aged ones, respectively.

(ii) The coercive force of ferromagnetic materials shows a similar dependence on the size of nano-scale coherent non-magnetic particles; there is, however, no over-aged state.

It is standard practice in metallography to derive the quoted geometric parameters of second phase particles from microscopic studies of the surface of the material. Generally some etching procedure is necessary to obtain satisfactory contrast. This holds with few exceptions for optical as well as for atomic force microscopy ( AFM ) [2-4]; also in scanning electron microscopy ( SEM ) [3,4] etching is helpful. Three of the few cases for which no etching is needed, are: optical

2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

**For Peer Review Only**

interference microscopy [5], some rare cases of AFM [2], and magnetic force microscopy of

ferromagnetic materials [3]. Chemical and electrolytic etching procedures take advantage of the fact that different phases are dissolved at different rates. Thermal etching works similarly [5]; ion beam etching, however, is more complex because knock-on processes and high-energy-density-zones have to be taken into consideration [6,7]. The surface relief created by etching can subsequently be imaged with satisfactory contrast. For the sake of clarity, up to the end of this section it is assumed that the particles dissolve faster than the matrix. But since the ratio of the dissolution rates of the particles and of the matrix is finite, also the matrix is attacked to some degree. Hence the pits marking the original positions of the etched away parts of the particles will be too large. This is called

over-etching, it may cause serious errors in the quantitative characterization of small particles.

In the progress of quantitative AFM and SEM characterizations of nano–scale plate-shaped
coherent precipitates of the disordered γ-phase in an L12-long range ordered γ’-matrix, the need arose
to relate the size of the etch-pits left behind by the etched away parts of the γ-precipitates to their
actual dimensions [3]. The overall chemical composition of the material was Ni69Co9Al18Ti4. The
main difference in the chemical compositions of the two phases is that the γ-plates are richer in
cobalt than the γ’-matrix. The arrangement of the two phases in Ni_{69}Co_{9}Al_{18}Ti_{4 }is inverse to that in
γ’-strengthened nickel-base superalloys, in which the disordered γ-phase forms the matrix and
particles of the L1_{2}-long range ordered γ’-phase precipitate [1,2,4,8]. The habit planes of the γ-plates
in Ni69Co9Al18Ti4 are of the type {001}. Preferential etching of the γ-plates occurred as a side effect
of the standard preparation procedure of thin foils for transmission electron microscopy ( TEM ):

twin-jet electrolytic polishing [3]. Without any further preparation specific to the applied microscope, the same foils were studied by AFM, SEM, and TEM.

Fig. 1 shows AFM-, SEM-, and TEM-images of such thin foils. The γ-pits left behind by the etched away parts of the plate-shaped γ-precipitates are clearly visible. The nominal indices of the macroscopic surface of the thin foil and hence of the image plane are (001). There are two families of edge-on γ-plates; the indices of their habit planes are (100) and (010). The in-plane γ-plates lie along (001). These micrographs will be discussed in detail in Section 3. In Figs. 1a and b quantitative information on AFM-imaged profiles of γ-pits is given. It is emphasized that measured AFM-profiles are determined by the actual shape of the γ-pits and by the geometry and inclination of the tip of the AFM [3]. The question was what were the actual size and shape of the γ-plates? To solve this

problem their size was also determined by TEM of thin foils and computer simulations of the etching

2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

**For Peer Review Only**

process were undertaken. The TEM study and the simulations proved that the actual size and shape of the γ-precipitates can be accurately derived from AFM-images of the γ-pits.

This former work was the starting point for a more general investigation of the etching processes
of two-phase materials: presently three-dimensional kinetic Monte Carlo simulations [9-11] were
performed. Both cases were treated: (i) the atomic binding energies in the particle are smaller than
those in the matrix, i.e. the particles dissolve faster than the matrix – as in Ni_{69}Co_{9}Al_{18}Ti_{4} – and (ii)
the opposite case, i.e. the matrix dissolves faster than the particles. The difference in dissolution rates
was varied widely. Three different particle shapes were considered. The procedures and the results
obtained are reported below. In Section 3.1 these results are compared with those of actually etching
γ-precipitates in Ni69Co9Al18Ti4.

**2. Modeling and simulations **

The modeled crystal structure, geometries, and etching procedures were as follows.

Throughout this communication the etchant will be supposed to be liquid, i.e. chemical and electrolytic etching are simulated. Simulations of thermal etching are quite similar.

*2.1. Crystal structures and geometries *

The specimen consists of two phases. Both, the particle as well as the matrix, are supposed to
*have the f. c. c. crystal structure, the same lattice constant a*_{0}, and to be fully coherent. Since in the
present model the number of neighboring atoms governs the dissolution rates of the atoms ( Section
2.2 ) and this number depends on the crystal structure, the latter has to be fixed. The simulation
procedures described below can easily be adapted to any other crystal structure.

The three most common particle shapes are treated: spheres, plates, and cubes with rounded edges and corners. Incidentally, the γ’-precipitates in advanced commercial γ’-strengthened

nickel-base superalloys are examples of such rounded cubes with edge lengths around 500nm [8].

The coordinates of the points on the matrix-particle phase boundary are given by Eq. (1); the center of the particle is at the origin of the coordinate system:

1

+ + =

*n* *n* *k*

*x* *y* *z*

α α β . (1)
This equation describes a superellipsoid [3,12,13]. The parameters α, β*, n, and k determine its shape. *

Eq. (1) is a unified convenient description of the geometry of all common convex particle shapes:

*spheres, cubes, plates, fibers. The z-axis has fourfold rotational symmetry and the three planes *
*characterized by x*

### ≡

*0, y*

### ≡

*0, and z*

### ≡

0 are mirror planes. There are two obvious generalizations of**For Peer Review Only**

*Eq. (1). The fourfold rotational symmetry of the z-axis can be reduced to a twofold one by replacing *
the two first terms in Eq. (1) by

### (

*x*/α1

### )

^{n}^{1}and

### (

*y*/α2

### )

^{n}^{2}

*, respectively, with n*1≠

*2 and / or α1≠*

^{n}^{α}2

*. Moreover, the mirror symmetry of the plane z*≡0 can be broken by assigning β

*and / or k*

*different values in the two half-spaces z>0 and z<0 [13].*

In the present simulations the following values are inserted for α, β*, n, and k; they yield the *
most common shapes of second phase particles:

*sphere: *α=β*=69.5a*_{0 }*, n=k=2 , *
plate: α*=69.5a*_{0 ,}β*=9.5a*_{0 }*, n=k=3 , *

*cube with rounded edges and corners: *α=β*=69.5a*_{0 }*, n=k=10 . *

*Evidently the maximum extensions of all three particles are the same along the [100]– and the [010]–*

*directions. Three–dimensional sketches are shown in Fig. 2. The exponents n=k=3 chosen for the *
plate are those found for the average plate-shaped γ-precipitate in Ni_{69}Co_{9}Al_{18}Ti_{4} [3] and the aspect
ratio α β/ =7 3. is close to that of the average γ-precipitate. However, the individual lengths α and β
quoted above for the modeled plate amount to only about one eighth of those of the average γ-plate.

It is emphasized that the γ-plates in Ni_{69}Co_{9}Al_{18}Ti_{4} had neither the shape of flat cylinders, nor of flat
cuboids, nor of flat standard ellipsoids, but that they could be very well described as superellipsoids
*with n=k=3 [3]. In the case of plate-shaped particles, etching along one of the two longer axes must *
be distinguished from etching along the short axis, i.e. the plates may be orientated either normal or
parallel to the original {001}-surface of the specimen. Correspondingly two different orientations of
the plate-shaped etch-pits must be distinguished: edge-on and in-plane orientation ( Fig. 1 ). The
*volume V of the superellipsoid is given by *

* V = q*V*(n,k) *π α^{2} β (2)
*with q*V*(2,2)=4/3=1.333 ( sphere ), q*V*(3,3)=1.813 ( plate ), and q*V(10,10)=2.443 ( rounded cube )
[3,13]. The habit plane of the plate and the sides of the rounded cube have the indices {001}.

The particle is embedded in a matrix-cube having {001}-surfaces. Its dimensions are:

0 0 0

350*a* × 350*a* × 350*a* . This cube and the spherical particle contain ≈172 10× ^{6} and
5 6 10. 6

≈ × atoms, respectively. Periodic boundary conditions are imposed such that an infinite

**For Peer Review Only**

*(001)-solid-etchant interface is created and etching is along the +z-direction. Only for the simulation *
of etching along the longer half-axis of the plate [ edge-on orientation ], this interface has the indices
*(010) and etching is along the +y-direction. It is tempting to make use of the symmetry of the system *
and to simulate only one quarter of it. But since this is not fully compatible with the random nature
of the dissolution process ( Section 3.1.2 ), it was presently not done. The centre of all particles has
the coordinates (0,0,0). With the only exception of the in-plane plate, the matrix-cube is centered at
*(0, 0, 174.5a*_{0} - α). In the case of the in-plane plate the centre of the matrix-cube is at

*(0, 0, 173a*0 - β ). Evidently, at the start of the simulations the sphere, the edge-on plate, and the
rounded cube are covered by just one atomic layer of matrix; in the case of the in-plane plate there
are four such layers.

*2.2. Modeling and simulations *

The activation energy for transferring an atom from the surface of the particle or from the
*surface of the matrix to the etchant is E*p* and E*m, respectively. These energies are assumed to be
proportional to the number ν * of first nearest neighbor atoms in the solid phases; hence E*_{p}* and E*_{m} are
low for atoms at edges and corners:

* E*p =

### ν

*e*p (3a)

*and E*

_{m }=

### ν

*e*

_{m}(3b) .

*Since the coefficients e*

_{p}

*and e*

_{m}are related to the energies required for breaking one first nearest

*neighbor bond in the particle or in the matrix, respectively, for simplicity in the following e*p

*and e*m

will be referred to as first nearest neighbor bond or binding energies. Of course, in the case of metals
the term “bond” is not quite appropriate. Effects of more distant neighbors will be discussed in
Section 2.4.2. All energies are normalized to kB*T, where k*B* is the Boltzmann constant and T the *
*absolute temperature. E*p* and E*m are calculated with Eqs. (3) even if some bonds cut through the
particle-matrix phase boundary; i.e. Eqs. (3) are applied irrespective of the fact that some of the
nearest neighbor atoms may be in the other solid phase. If, however, the fraction of particle atoms
which have nearest neighbors in the matrix, is appreciable, bonds crossing the phase boundary must
*be assigned energies which differ from e*p* and e*m. This will be necessary if the extension of the
particle in one or more directions is very small; i.e. if the particle is very small or if the plate is very
thin. Phases consisting out of more than one type of atoms are referred to in Section 2.4; for such
*materials e*p* and e*m in Eqs. (3) may be considered as suitable averages.

The number ν of the present (001)- and (010)-solid-etchant interfaces of the three dimensional f. c. c. crystal ranges from four for an add-on atom to eight for an atom in a perfect

**For Peer Review Only**

{001}-interface, whereas ν * of a two dimensional simple square lattice varies only between one and *
three. Evidently, realistic results can only be derived from simulations of three-dimensional crystals.

*The range of e*p* and e*m covered in the present kinetic Monte Carlo simulations is 1.0-3.4 and
*the ratio e*m*/e*p* is between 1/1.3 and 1.3. This range of e*p* and e*m is close to the one covered by Strobel
et al. [14] in their kinetic Monte Carlo simulations of Ostwald ripening. Moreover the present highest
*value 3.4 is close to one half of the actual, normalized ( to k*B*T, T=300K ) bulk first nearest neighbor *
pair-interaction energies

### ε

_{Cu 1}and

### ε

_{Ni 1}of copper and nickel, respectively. In Table 1 the values of

### ε

Cu j and### ε

_{Ni j}

*, 1<j<3, of the first three coordination shells are listed.*

### ε

_{Cu j}and

### ε

_{Ni j}were derived from the pair potential functions published by Mishin et al. [15,16] by inserting the respective shell

*radii r*j. The quoted authors have shown that lattice properties calculated on the basis of their pair potential functions agree well with experimental data.

*Since only the N atoms at the surface of the solid can be dissolved, only they are considered. *

At the start of the kinetic Monte Carlo simulation the solid-etchant interface is a perfect (001)-plane
*[ (010)-plane for the edge-on plate ] with N*≈0.25×10^{6} atoms. As stated above, etching is along the
*+z-direction [ along the +y-direction for the edge-on plate ]. The simulation of the dissolution of one *
atom will be referred to as one step; each step involves three sub-steps:

(i) *With the aid of Eqs. (3) the relative, non-normalized thermodynamic probability p*i of the
*dissolution of atom No. i is calculated. This is done for all N interface atoms. Eqs. (4a) *
and (4b) hold for particle and matrix atoms, respectively:

*p*

_{i}

### = e

^{−}

^{−−}

^{−}

^{E}^{p , i}(4a) and

*p*

_{i}

### = e

^{−}

^{−−}

^{−}

^{E}^{m, i}, (4b)

*1 ≤ i ≤ N. The pre-exponential factors of both phases are assumed to be the same; hence *
these factors are disregarded.

(ii) The ratio*s*_{µ}, 1 ≤ *µ ≤ N, is calculated *

*s*_{µ} = j j

=1 =1

### ∑

^{µ}

### ∑

*j* *j*

*p* *p*

Ν

. (5)

*s*

0*is zero and*

*s*

N equals unity.
(iii) *A uniform random number w, 0 ≤ w ≤ 1, is generated and the atom No. n, 1 ≤ n ≤ N, for *

**For Peer Review Only**

*which s*n-1*<w ≤ s*n holds, is transferred from the solid to the etchant.

*Evidently the probability that atom No. n is dissolved in this step equals * _{n} _{j}

=1

/

### ∑

^{N}*j*

*p* *p* . Subsequently the
next step is started for the new solid-etchant interface, which differs from the previous one, because
one atom has been removed in the previous step. Exactly one atom is dissolved in each step. The
*total number of steps required to entirely dissolve the particle depends on its shape and on e*_{p}* and e*_{m}.
*This will be demonstrated in the figures presented in the following section. *

*2.3. Results of the kinetic Monte Carlo simulations *

A choice of simulation results is presented in Figs. 3-8. Throughout the following the term

*“front of etching” refers to the most advanced point of the solid-etchant interface. If e*_{p} is smaller
*than e*_{m}*, the particle dissolves faster than the matrix and vice versa. In the latter case, e*_{p}*>e*_{m}, during
intermediate stages of etching the particle protects the matrix lying directly under it from the attack
by the etchant ( Figs. 3, 5, 6h ), but finally the particle becomes completely detached from the matrix.

In Figs. 3-5 dark grey lines outline the periphery of such free particles. Animations of simulated
etching processes are available for all presently studied particle shapes and for two combinations of
*normalized binding energies: e*_{p}*=1.70, e*_{m}*=2.21 and e*_{p}*=2.21, e*_{m}*=1.70 [17]. The effects of varying the *
*ratio e*_{m}*/e*_{p}* of the normalized binding energies, while keeping e*_{m} constant, are demonstrated in Fig. 7
for the spherical particle. Since Eqs. (4) are non-linear the etched profile does not only depend on the
*ratio e*_{m}*/e*_{p}*, but also on the individual values e*_{p}* and e*_{m}*; this is shown in Fig. 8 for e*_{m}*/e*_{p}≡1.15. Fig. 8
*demonstrates what happens if the temperature T is varied while the non-normalized ( to k*B*T ) *
*activation energies for dissolution are kept constant: T decreases from Fig. 8a to 8f. From Figs. 3-8 *
the following results are extracted. Though not all of them can be proved within reasonable times for
*all combinations of e*p* and e*m* in the entire range 1.0 < e*p*, e*m < 3.4 presently studied, all listed results
are considered as reliable. This is emphasized for results Nos. A2) and A3). Results Nos. A1), A5),
B1), B2.1), B2.2), and B2.4) are direct consequences of Eqs. (3), according to which the activation
energy for the dissolution of an atom is proportional to the number

### ν

of its first nearest neighbors:### ν

of atoms at edges and corners is relatively low and high in the most densely packed {111}-planes.

**Results: **

A) General

A1) The roughness of the solid-etchant interface is low: plus / minus 1-2 atomic diameters ( see B2.1) below ). This can be inferred from Fig. 6 and from the animations [17]. Moreover it is indicated by the small wiggles of the curves representing the interface in Figs. 3-5, 7, and 8.

**For Peer Review Only**

A2) Over-etching is quite frequently observed: if the particle dissolves faster than

the matrix, the resulting etch-pit is too large and in the opposite case the remainder of the
particle, which sticks out of the matrix, is too small. In intermediate stages of etching the
solid-etchant interface stays the closer to the original matrix-particle phase boundary the
larger the term *e*_{p} −*e*_{m} * is ( see also B2.3) below ). If the ratio e*_{m}*/e*_{p} is smaller than 1/1.3 or
larger than 1.3 and etching does not continue too long, over-etching is almost negligible
( Figs. 3-5 ) for all particle shapes and orientations presently considered. If after etching the
largest extension of the original particle is not close to the surface of the specimen, the size of
the particle may be underestimated ( Figs. 3 and 4 ).

A3) *Even if e*p* and e*m differ by as little as 5%, etching reveals a spherical particle ( Figs. 7c, d ).

Though no simulations have been performed to establish analogous limits for the other particle shapes, it is expected that similar limits apply also for them.

A4) *Due to the non-linearity of Eqs. (4) the etched profiles do not only depend on the ratio e*m*/e*p

*but also on the individual values of e*p* and e*m. This dependence is strongest if both bond
energies are rather low ( Fig. 8 ).

A5) Far away from the particle, respectively from the etch-pit, the matrix is planar - except for steps of atomic height - and follows (001)-planes [ (010)-planes for the edge-on plate ]; this proves that the matrix-cube is sufficiently large.

B) *The particle dissolves faster than the matrix: e*p*<e*m

B1) At the very beginning of etching several small shallow pits appear. Later they

coalesce and a single deep pit is formed at the original site of the particle ( e.g. Figs. 5a and b, animation [17], and Section 3.1.2 ). This primarily concerns the rounded cube and the

in-plane plate, which have an almost flat, respectively a rather flat top interface with the etchant.

B2) After an appreciable amount of the particle has dissolved, several different types of particle-etchant interfaces can be distinguished:

B2.1) Much of the interface is along terraces of the most densely packed {111}-planes. This can be
*seen best in Figs. 3 and 6 and in the animations [17]. In Figs. 3a and b showing the sphere, *
the traces of the solid-etchant interface are along the [101]-direction, which lies in the

intersection of the

### ( )

111 -plane with the### ( )

111 -plane, and along the [101]-direction, which lies in the intersection of the### ( )

^{111}-plane with the

### ( )

111 -plane. In the pseudo-three-dimensional presentation of the cubic particle shown in Fig. 6c two families of {111}-planes are visible;**For Peer Review Only**

the other two families of {111}-planes are in the cut away front half of the matrix-cube. The
height of the steps between adjacent {111}-terraces is of atomic dimensions. At constant ratio
*e*m*/e*p the predominance of {111}-planes is most pronounced if the normalized binding

*energies e*m* and e*p * are high, i.e. the temperature is low ( Fig. 8 ). The reason for this energy *
dependence is the non-linearity of Eqs. (4).

B2.2) The central area of the bottom solid-etchant interface of a partially dissolved cubic particle is along (001)-planes ( e.g. Figs. 3e, f and 6c ).

B2.3) When the solid-etchant interface reaches the particle-matrix phase boundary, etching slows
*down drastically because from then on it is governed by e*m*, which is higher than e*p. Hence
this interface stays close to the original phase boundary, see e.g. the upper part of the
spherical particle in Fig. 3a and the sides of the rounded cube in Fig. 3e.

B2.4) After the entire spherical particle and an appreciable amount of the matrix below the original position of the particle have been dissolved, much of the surface of the etch-pit is formed by {111}-and {001}-planes ( Fig. 3 ). A pit remains discernable for very long etching times.

C) *The matrix dissolves faster than the particle: e*p*>e*m

C1) The most conspicuous effect has already been mentioned: at intermediate stages of etching the particle protects the matrix lying directly under it from the attack by the etchant, but later the particle completely loses contact to the matrix ( Figs. 3, 5, 6h ). As to be expected it is the in-plane plate which becomes detached from the matrix at the lowest total number of

dissolved atoms. After a particle has become free, during further etching all traces of it in the surface of the matrix disappear very soon.

C2) Etching exposes different families of crystallographic planes of the spherical particle. This is
*easily noticeable for e*_{m}*=1.92 and e*_{p}*=2.21 in Fig. 3d. If the difference between e*_{p}* and e*_{m} is
*larger, e.g. e*_{m}*=1.70 and e*_{p}=2.21 in Fig. 3c, the sphere becomes completely free before it
changes its shape markedly. The analogous effects for the rounded cube are less pronounced
because planes close to {001} persist for long times of etching ( Figs. 3g, h ).

C3) *For e*_{p}*>e*_{m}*, the front of etching proceeds much more slowly than for e*_{p}*<e*_{m} ( see B) above )
because most of the top area of the matrix is rather flat and much more atoms must be
dissolved before the same maximum depth is reached ( Figs. 3-5).

*2.4. Secondary effects *

There are several processes which may affect etching beyond that which has been considered so far. Seven of them are listed here and the two first ones will be analyzed in the subsequent sections:

**For Peer Review Only**

(i) After a particle which dissolves faster than the matrix, has been etched very deeply it becomes difficult to provide fresh etchant at the bottom of the pit and to remove the dissolved atoms from it.

The ensuing effects will be analyzed in Section 2.4.1.

(ii) The possible effects of second and third nearest neighbor bonds have already been referred to and will be discussed in Section 2.4.2.

(iii) The number ν of first nearest neighbor atoms depends on the crystallographic orientation of the solid-etchant interface, e.g. ν equals eight for the perfect {001}- and nine for the perfect

{111}-interface ( Table 1 ). Hence the etching process may vary with the orientation of the original interface.

*(iv) The binding energies e*p* and e*m may vary with ν . This can be modeled by adding higher order
terms of ν on the right hand sides of Eqs. (3).

(v) In Section 2.2 it has already been mentioned that in the case of very small particles and very thin
plates it will be appropriate to allow for the fact that bonds which cut through the particle-matrix
*phase boundary have energies which differ from e*_{p}* and e*_{m}.

(vi) If a particle which dissolves faster than the matrix, is surrounded by a strain field, over-etching is
*likely to occur. This can be simulated by lowering e*m in the region of the strain field.

(vii) In general the matrix as well as the particle will consist out of more than one type of atoms. This
*can be allowed for when the crystal is built up in the computer. In such cases e*p* and e*m depend on the
types of neighboring atoms. This point is of importance for long range ordered phases; for them the
*present normalized energies e*p* and e*m may be considered as averages.

*2.4.1. Effects of a lack of fresh etchant in the etch-pit *

If the etch-pit left behind by the etched away parts of a particle which dissolves faster than the matrix, is narrow and deep it becomes difficult to provide fresh etchant at the bottom of the pit and to remove the dissolved atoms from it. The relevant processes are governed by a host of parameters:

e.g. shape and size of the pit, convection and diffusion of the etching agent and of the dissolved
atoms, viscosity of the etchant, its adhesion to the solid. As mentioned, the ensuing effects become
serious if the pit is deep and narrow or has a bottle neck at its top. Such a neck is formed e.g. if the
*particle has the shape of a sphere and the binding energy e*p* is appreciably smaller than e*m ( Figs. 3a
and 6a). Instead of attempting to take all relevant processes into consideration just the two basic
features of the hindrances to the etching process are allowed for in the present kinetic Monte Carlo
simulations for a spherical particle: the narrower the upper part of the pit is and the deeper it is, the
more significant are these hindrances.

**For Peer Review Only**

*The mathematical formulation for etching along the z-direction is as follows. The coordinates *
*of all atoms are integer multiples of ½a*0*, where a*0 is the lattice constant. To calculate the

*non-normalized probability p*1 ( Eqs. (4) ) of dissolving the atom ( particle or matrix atom ) having
*the coordinates (x*1*, y*1*, z*1), the right hand sides of Eqs. (4) are multiplied by the function

### Φ

( )*z*

_{1},

*which is related to the probability that the etchant agent penetrates to the depth z*1

*:*

### Φ

( )*z*

_{1}= exp

### {

^{-}

^{λ z}^{(}

^{1}

^{-}

^{z}^{m}

^{) /}

^{2}

^{A}### }

for (*z*

_{1}-

*z*

_{m})

*>a*0

(6) and

### Φ

( )*z*

_{1}= 1.0 for (

*z*

_{1}-

*z*

_{m}) ≤

*a*

_{0}, where

### λ

*is a numerical coefficient, z*

_{m}

*the average z-level of the matrix far away from the pit where*

*the matrix is planar, and A is an average over the area of all cross-sections of the pit with z*

_{m}

*<z<z*

_{1}:

= ^{=}

−

### ∑

_{j}

^{z a}

_{z a}

^{S}

A z z a

1 0

m 0

2 / *

2 / j

1 m 0

2( ) / . (7)
*To allow for a bottle neck of the pit, not the actual cross-section at the level z= ja*_{0}/2 is inserted into
the sum, but *S*^{*}_{j}*, which is the minimum area of all cross-sections with z*m*<z< ja*0/2. If the pit narrows
*continuously as z increases, A is the arithmetic mean cross-section. The limitations *(*z*_{1}-*z*_{m})*>a*_{0} and

1 m

(*z* - *z* ) ≤*a*_{0} in Eq. (6) have two consequences: (i)

### Φ

( )*z*

_{1}is not affected by the roughness of the solid-etchant interface ( Section 2.3 ) and (ii)

### Φ

( )*z*

_{1}is smaller than unity only if the respective atom lies in the surface of the etch-pit. Two alternative values are inserted for the coefficient

### λ

*: 0.2 and*1.0. For

### λ

= 0*, the standard results presented in Section 2.3 and Fig. 3 are recovered. Evidently the*effects of a lack of fresh etchant are the more serious the larger the extension of the the particle along

*the z-direction is. The results for the spherical particle and e*p

*=1.70 and e*m=2.21 are shown in Fig. 9.

As the ratio

### {

^{(}

^{z}^{1}

^{-}

^{z}^{m}

^{) /}

^{2}

^{A}### }

increases,### Φ

( )*z*

_{1}becomes small and the advancement of the front of etching slows down. This effect is the stronger the larger

### λ

is. A comparison of Fig. 3a with Fig. 9 leads to the following conclusions:(1) Due to the term (*z*_{1} -*z*_{m})^{2} in Eq. (6), for

### λ

>0 the (001)–bottom of the etch-pit is flat and*wide. This effect is enhanced by small areas A.*

(2) At a given position of the front of etching in the particle, i.e. at given value of δ in Figs. 3a and 9, the number of dissolved atoms increases drastically with

### λ

.**For Peer Review Only**

(3) The larger

### λ

is, the more matrix atoms next to the original particle-matrix phase boundary dissolve before the front of etching reaches the bottom of the particle. As to be expected this enhances over-etching.*2.4.2. Effects of interactions with second and third nearest neighbor atoms *

So far only the interactions with first nearest neighbor atoms have been taken into

consideration in the kinetic Monte Carlo simulations. In this section the effects of second and third
nearest neighbor interactions are analyzed. Besides the normalized first nearest neighbor bond
*energies e*p* and e*m, the respective second nearest neighbor energies *e*^{*}_{p} and *e*^{*}_{m} and the third nearest
neighbor energies *e*^{**}_{p} and *e*^{**}_{m} * are allowed for. Eqs. (3a) and (3b) for the activation energies E*_{p} and
*E*m for dissolution are replaced by Eqs. (8a) and (8b), respectively:

* E*p = *ν e*_{p}+ *ν e*^{* *}_{p} + *ν e*^{** **}_{p} (8a)
*and E*_{m }= *ν e*_{m}+ *ν e*^{* *}_{m} + *ν e*^{** **}_{m} , (8b)
where

### ν

_{, }

### ν

^{∗}

_{, and }

### ν

^{*}

^{*}are the numbers of first, second, and third nearest neighbor atoms,

respectively. Introducing the ratios *e*_{p}^{/}*e*^{*}_{p}^{=}

### ρ

_{p1},

*e*

_{m}

^{/}

*e*

^{*}

_{m}

^{= }

### ρ

_{m1}

*, e*

_{p}

^{/}

*e*

^{**}

_{p}

^{=}

### ρ

_{p2}, and

*e*

_{m}

^{/}

*e*

^{**}

_{m}

^{=}

### ρ

_{m2}

into Eqs. 8(a) and 8(b) yields

* E*p* = e*p (

### ν

+ ν^{*}/ρ +

_{p1}ν

^{**}/ ρ ) (8c)

_{p2}

*and E*m

*= e*m (

### ν

+ ν^{*}/ ρ

_{m1}+ ν

^{**}/ ρ

_{m2}) . (8d) For the sake of argument the ratios

### ρ

_{p1},

### ρ

_{m1},

### ρ

_{p2}, and

### ρ

_{m2}are related to the normalized pair interaction energies

### ε

_{Cu j}

*, 1<j<3, of copper introduced in Section 2.2 and listed in Table 1:*

### ρ

p1=### ρ

_{m1}=

### ε

_{Cu 1}/

### ε

_{Cu 2}= 3.36 and

### ρ

_{p2}=

### ρ

_{m2}=

### ε

_{Cu 1}/

### ε

_{Cu 3}= 24.9. Evidently, allowing for the interactions with second and third nearest neighbors is equivalent to raising the effective number of

*first nearest neighbors. The additional terms may seem small. p*

_{i }, which governs the probability of dissolving an atom ( Eqs. (3) and (4) ), is, however, lowered by the factors

*exp[ - e*p (ν^{*} / 3.36 + ν^{**} / 24.9)] and * exp[ - e*m (ν^{*} / 3.36 + ν^{**} / 24.9)], respectively. For a
*perfect {001}-plane and e*_{p}*=1.70, this factor amounts to 1/28.5 and for e*_{m}=2.21 it is 1/77.8 .

Allowing for second and third nearest neighbor interactions has the effect of amplifying the difference in the dissolution probabilities brought about by the first nearest neighbor interactions.

**For Peer Review Only**

Moreover, ν^{*} and ν^{**} tend to increase with ν: an atom located at an edge or corner has relatively
few first nearest neighbors as well as relatively few more distant ones.

Interactions with more distant neighbors affect {111}- and {001}-planes to different degrees.

Let *E*( , *µ hkl*)* be the activation energy for the dissolution of an atom in a perfect {hkl}-plane and *µ
is the number of coordination shells allowed for. The ratios *E*(1, 111) /*E*(1, 001),

(2, 111) / (2, 001),

*E* *E* and *E*(3, 111) /*E*(3, 001) equal 1.13, 1.04, and 1.05, respectively. They
decrease as µ increases, but not monotonically. This non-monotonic variation of these ratios with µ
is not caused by the present choice of ρ_{pi} and ρ_{mi}, but by the dependence of ν^{*} and ν^{**} on the
*indices {hkl}. E*(1, 111) /*E*(1, 001) > *E*(3, 111) /*E*(3, 001) > *E*(2, 111) /*E*(2, 001) holds for

2 1 0

1.75ρ > ρ > .

*Some results of the simulations for a spherical particle with e*_{p}*=1.92 and e*_{m}=2.21 are
presented in Fig. 10. There both cases are shown: allowing (i) for first and second and (ii) for first,
second, and third nearest neighbor bonds. These simulations are very time consuming. The most
important result is that unless the particle has been completely dissolved, the width of the top of the
etch-pit is nearly independent of the number µ, i.e. over-etching is independent of µ. Again {111}-
and {001}-planes are exposed. The interactions with more distant neighbor atoms flatten the

(001)-bottom of the etch-pit in the particle; this effect is similar to that of a lack of fresh etchant at
the bottom of the etch-pit ( Fig. 9, Section 2.4.1 ). The width of the (001)-bottom does not increase
monotonically with µ: the bottom is widest for µ= 2. This is tentatively interpreted to be due to
the above stated variation of the ratios of the {111}- and {001}-activation energies with µ: as µ is
raised, they approach each other, but not monotonically. Low ratios *E*(µ, 111) / (*E* µ, 001) favor the
exposure ( not the dissolution rate! ) of {001}-planes and thus widen the (001)-bottom of the
etch-pit. As long as the particle has not completely dissolved, the numbers ω_{2} and ω_{3} of dissolved
atoms ( Fig. 10 ) are smaller than ω_{1}. There are two mechanisms which contribute to this effect: (i)
the amplification of differences in dissolution rates for µ>1 mentioned above in connection with
Eqs. (8) and (ii) the variation of the ratio *E*( , 111) /µ *E*( , 001)µ with µ, due to which the dissolution
rate of atoms in the (001)-matrix-surface is less favored for µ>1 than for µ=1. Hence relative fewer
atoms of this (001)-matrix-surface are dissolved for µ>1. Since its area is large, this effect

outweighs that of widening the etch-pit.

**For Peer Review Only**

**3. Discussion: Comparison of Monte Carlo Simulation with TEM Results **

Most of the results of the kinetic Monte Carlo simulations of etching have already been
discussed in Sections 2.3 and 2.4. However, it remains to relate them to the etching experiments
carried out for the plate-shaped precipitates of the γ-phase in Ni69Co9Al18Ti4 [3] ( Section 1 ). AFM-,
SEM-, and TEM-images of them are presented in Fig. 1. Since the γ-plates dissolve faster than the
*γ’-matrix, etching produces γ-pits. Hence in Sections 3.1 and 3.2 only the case e*m*>e*_{p }is considered.

The three types of microscopes yield complementary information; quantitative data on the depth
profile of the γ-pits are most easily obtained by AFM. If the slope of the surface relief of the
specimen changes abruptly, the geometry and the inclination of the tip of the AFM must be taken
into consideration [3] ( Section 1 ). It turned out to be very difficult to unambiguously determine the
real shape of the plate-like γ-precipitates in Ni_{69}Co_{9}Al_{18}Ti_{4} by using the experimental data of only
one of the three applied microscopic methods [3]. If, however, the data obtained by one microscope
are complemented by computer simulations of the etching process, the reliable characterization of
the γ-precipitates is possible. In Sections 3.1.2 and 3.2 the actual shapes of the γ-precipitates and of
the γ-pits will be derived from the micrographs and subsequently these shapes will be discussed with
reference to the respective relieves obtained in the simulations. The original surface of the specimen
is parallel to (001).

*3.1 In-plane *γ*-plates *

The AFM-, SEM-, and TEM-images of in-plane γ-pits in Ni69Co9Al18Ti4 shown in Fig. 1 deviate somewhat from perfect four-fold rotational symmetry. There are two groups of entirely different effects which may give rise to asymmetries: (i) the two longer axes of the γ-plates

themselves may differ in length and (ii) etching may produce asymmetric γ-pits even if the γ-plates are perfectly symmetric. These two groups are discussed in the following.

*3.1.1 Asymmetry of the *γ*-plates *

The growth rate of each γ-plate in Ni69Co9Al18Ti4 is governed by the surrounding

concentration gradients of the precipitating elements. These gradients are affected by neighboring
γ-plates, the nucleation of which occurs at random. Hence the growth rate of in-plane γ-plates may be
different along the [100]- and along the [010]-direction. The average difference in length of the two
longer half-axes of the in-plane γ-plates was experimentally found to be ±_{1 0 %} [3].

*3.1.2 Asymmetric etching *

**For Peer Review Only**

Since the aspect ratio α/β ( =longer axis / shorter axis ) of the majority of the γ-plates in
Ni_{69}Co_{9}Al_{18}Ti_{4} exceeds 7.0 [3], even minor deviations of the actual orientation of the surface of the
macroscopic specimen from the exact nominal (001) one have strong effects on the appearance of
**in-plane γ-pits. The γ-pit marked B in Fig. 1a is an example. For a cuboidal pit with the aspect ratio **

### β

### α

/ =7.0, a deviation as small as 8.1° from the nominal orientation leads to a depth error=α

*∆t* tg8.1°=β **. The inclination of the bottom of the γ-pit marked B in Fig. 1a amounts to about **
3.3°; this angle was calculated from the depth profile shown in the upper right of Fig. 1a. It is for
**such a misorientation that the right corner of B is missing. Due to an inclination of the γ-pit relative **
to the macroscopic surface of the specimen, in the SEM the yields of secondary electrons from
opposite - ascending and descending - slopes of the in-plane γ-pit are different. Hence the two slopes
appear at different brightness in the micrographs: the upper rims of the γ-pits in Figs. 1c and d are
much brighter than the lower ones. There are at least three reasons for deviations of the orientation of
the macroscopic surface from (001): (i) errors in cutting the slice from which the thin TEM-foil is
prepared, (ii) small angle boundaries in the foil, and (iii) after its electro-polish, its surface is slightly
concave. Since the γ-plate is slightly convex ( Fig. 2 ), in a perfectly well orientated specimen the
first contact of the etchant with the in-plane γ-plate is most likely to occur at its apex. Hence the
dissolution of the γ-plate proceeds from its center towards its corners.

The contrast of secondary electron images primarily depends on the orientation of the surface of the specimen relative to the incident electron beam. Therefore the ascents and descends of

in-plane γ-pits yield strong contrast in the SEM. The AFM shows the topography of the specimen,
i.e. the contrast is governed by differences in height. In the TEM, however, two entirely different
mechanisms strongly contribute to the contrast: strain contrast and thickness contrast [3]. Since the
average atomic numbers of both phases in Ni69Co9Al18Ti4 are nearly the same, there is hardly any
atomic number contrast. Strain contrast renders the not yet dissolved parts of partially dissolved
*in-plane γ-plates visible. Even if an in-plane γ-plate is completely embedded in the γ’-matrix and has *
no contact with either surface of the foil, the γ-plate may produce strain contrast. At γ-pits the local
thickness of the TEM-foil is reduced and thickness contrast is generated.

The white arrows in the SEM-images presented in Figs. 1c and d point at missing corners of the in-plane γ-pits; there their outline is parallel to <011>- instead of to <001>-directions. The reason for these missing corners is that the in-plane γ-precipitates have been dissolved only partially;

actually in the apparently missing corners some γ-pockets are still left. Due to their strain contrast they are visible in the TEM. In the AFM and SEM, however, such corners remain invisible. The top